The Alloy Tree: A Guide to Low-alloy Steels, Stainless Steels and Nickel-base Alloys
Embed Size (px)
Text of The Alloy Tree: A Guide to Low-alloy Steels, Stainless Steels and Nickel-base Alloys
This page intentionally left blank
The alloy tree A guide to low-alloy steels, stainless steels and nickel-base alloys
J. C. M. Farrar
Published by Woodhead Publishing Limited, Abington Hall, Abington Cambridge CB1 6AH, England www.woodhead-publishing.com
Published in North America by CRC Press LLC, 2000 Corporate Blvd, NW Boca Raton FL 33431, USA
First published 2004, Woodhead Publishing Limited and CRC Press LLC © 2004, Woodhead Publishing Ltd
This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. Reasonable efforts have been made to publish reliable data and information, but the author and the publishers cannot assume responsibility for the validity of all materials. Neither the author nor the publishers, nor anyone else associated with this publication, shall be liable for any loss, damage or liability directly or indirectly caused or alleged to be caused by this book.
Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming and recording, or by any information storage or retrieval system, without permission in writing from the publishers.
The consent of Woodhead Publishing Limited and CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from Woodhead Publishing Limited or CRC Press for such copying.
Trademark notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe.
British Library Cataloguing in Publication Data A catalog record for this book is available from the British Library.
Library of Congress Cataloguing in Publication Data A catalog record for this book is available from the Library of Congress.
Woodhead Publishing ISBN 1 85573 766 3 CRC Press ISBN 0-8493-2575-7 CRC Press order number: WP2575
Typeset by SNP Best-set Typesetter Ltd., Hong Kong Printed by TJ International, Padstow, Cornwall, England
Preface ix Acknowledgements x How to use this guide xi
Group A Creep-resisting low-alloy steels 1 Introduction 3 A–0 0.2% carbon, 1% manganese, 0.5% molybdenum fine- grained elevated temperature steel 4 A–1 11/4% chromium–1/2% molybdenum and 21/4% chromium–1% molybdenum creep-resisting steels 6 A–2 5% chromium–1/2% molybdenum and 9% chromium–1% molybdenum creep-resisting steels 8 A–3 Modified 9% chromium, 1% molybdenum creep-resisting steel 10 A–4 Modified 9% chromium, 1% molybdenum creep-resisting steel with tungsten 12 A–5 1/2–3% chromium, 1/2–1% molybdenum, 1/4% vanadium creep-resisting steels 14 A–6 21/4%–21/2% chromium plus alloying creep-resisting steels 16 A–7 12% chromium, molybdenum, vanadium creep-resisting steel 18 A–8 Modified 12% chromium, 0.5% molybdenum, 2% tungsten creep-resisting steel 20
Group B Cryogenic, nickel low-alloy steels 23 Introduction 25 B–0 0.2% carbon, 1.5% manganese fine-grained structural steel 26 B–1 1.5%–3.5% nickel cryogenic steels 28 B–2 9% nickel cryogenic steels 30
Group C Martensitic and ferritic stainless steels 33 Introduction 35 C–0 Plain 11–12% chromium steels with very low carbon contents and little additional alloying 36 C–1 Plain 11–13% chromium martensitic steels with various carbon contents 38
C–2 Plain 17% chromium ferritic stainless steels 40 C–3 Plain 26% chromium ferritic stainless steel 42 C–4 14–17% chromium, 5% nickel, 2–3% copper, precipitation-hardening stainless steels 44 C–5 Low-carbon 13% chromium steels with 4.5% nickel and 1.5% molybdenum 46 C–6 Extra low-carbon 11–13% chromium steels with various levels of nickel and molybdenum 48 C–7 Extra low-carbon, 29% chromium, 4% molybdenum superferritic stainless steel 50
Group D Duplex and superduplex stainless steels 53 Introduction 55 D–0 Lean alloy duplex stainless steels 56 D–1 22% chromium, standard duplex stainless steels 58 D–2 25% chromium, superduplex stainless steels 60 D–3 25% chromium, superduplex stainless steels with copper and/or tungsten 62
Group E Standard austenitic stainless steels 65 Introduction 67 E–0 18% chromium, 8% nickel austenitic stainless steels, stabilised with titanium or niobium 68 E–1 18% chromium, 8% nickel standard austenitic stainless steel 70 E–2 18% chromium, 8% nickel austenitic stainless steel with controlled carbon content 72 E–3 17% chromium, 12% nickel, 2.5% molybdenum austenitic stainless steel 74 E–4 Austenitic stainless steels with high manganese and nitrogen 76
Group F Austenitic and superaustenitic stainless steels 79 Introduction 81 F–0 19% chromium, 13% nickel, 3.5% molybdenum, austenitic stainless steel 82 F–1 Very low-carbon, 25% chromium, 20% nickel, austenitic stainless steels 84 F–2 21% chromium, 26% nickel, 5% molybdenum, 2% copper austenitic stainless steel 86 F–3 6% molybdenum, nitrogen-alloyed superaustenitic stainless steels 88 F–4 Superalloyed, high-nitrogen austenitic stainless steels 90
F–5 20% chromium, 34% nickel, 2.5% molybdenum, 3.5% copper plus niobium, austenitic stainless steel 92 F–6 22% chromium, 42% nickel, 3% molybdenum, 2.5% copper plus titanium, nickel alloy 94
Group G Corrosion-resistant nickel alloys 97 Introduction 99 G–0 22% chromium, 62% nickel, 9% molybdenum, 3.5% niobium, nickel alloy 100 G–1 17% chromium, 55% nickel, 16% molybdenum, 4% tungsten, nickel alloy 102 G–2 16% chromium, 57% nickel, 16% molybdenum, 4% tungsten, nickel alloy 104 G–3 22% chromium, 56% nickel, 13% molybdenum, 3% tungsten, nickel alloy 106 G–4 22% chromium, 16% molybdenum, nickel alloys, with and without copper and tungsten 108 G–5 28% chromium, 30% nickel, 3.5% molybdenum, 1% copper plus nitrogen, nickel alloy 110 G–6 30% chromium, 44% nickel, 5.5% molybdenum, 2% copper plus tungsten and niobium, nickel alloy 112 G–7 29% chromium, 61% nickel, nickel alloy 114
Group H Heat-resistant stainless steels 117 Introduction 119 H–0 Controlled carbon, 17% chromium, 12% nickel, 2.5% molybdenum austenitic stainless steel 120 H–1 15% chromium, 10% nickel, 1% molybdenum, 6% manganese austenitic stainless steel with vanadium, niobium and boron additions 122 H–2 21% chromium, 11% nickel, austenitic stainless steel with controlled carbon content, silicon, nitrogen and REM 124 H–3 18% chromium, 8% nickel, austenitic stainless steel with controlled carbon content 126 H–4 Medium carbon, 25% chromium, 20% nickel, austenitic stainless steels 128 H–5 Low carbon, 18% chromium, 38% nickel, 2% silicon, austenitic stainless steels 130 H–6 High carbon, 17% chromium, 38% nickel, austenitic stainless steel 132 H–7 0.4% carbon, 25% chromium, 20% nickel, cast austenitic stainless steels 134 H–8 0.4% carbon, 25% chromium, 35% nickel, cast austenitic stainless alloys 136
H–9 0.5% carbon, 25–28% chromium, 35–50% nickel, 0–15% cobalt, 5% tungsten, cast austenitic alloys 138 H–10 0.4% carbon, 35% chromium, 45% nickel, cast austenitic alloys 140 H–11 50% chromium, 50% nickel, 2% niobium, cast austenitic alloy 142
Group I Heat-resistant nickel alloys 145 Introduction 147 I–0 Controlled carbon, 21% chromium, 32% nickel, with aluminium and titanium, iron–base alloy 148 I–1 75% nickel, 16% chromium, 8% iron, nickel alloy 150 I–2 28% chromium, 45% nickel, 23% iron, 3% silicon with REM additions, nickel alloy 152 I–3 25% chromium, 46% nickel, 3% molybdenum, 3% cobalt, 3% tungsten, nickel alloy with 1% silicon 154 I–4 22% chromium, 54% nickel, 9% molybdenum, 12% cobalt, plus aluminium, nickel alloy 156 I–5 22% chromium, 47% nickel, 9% molybdenum, 2% cobalt with tungsten, aluminium and titanium, nickel alloy 158
Group J Nickel, nickel–copper and nickel–molybdenum alloys 161 Introduction 163 J–0 Pure nickel 164 J–1 65% nickel, 30% copper alloy 166 J–2 Copper with 10–45% nickel alloys 168 J–3 Nickel alloys with 28% molybdenum and small additions of iron and chromium 170
Appendix 1: Abbreviations 172 Appendix 2: Specifications 174 Appendix 3: Product forms 177 Appendix 4: Alloying costs 178 Appendix 5: The role of individual elements 180 Appendix 6: Types of corrosion 185
Bibliography and sources of further information 187
Index of generic numbers 191
In 1984, a small group in the technical department at Metrode Products Ltd produced a design for a wall chart that illustrated the evolutionary nature of the various alloyed welding consumables which formed the basis of Metrode’s product range. The chart was always referred to as ‘The Alloy Tree’ because the main trunks, side branches and smaller branches that showed the development of various alloy groups resembled a tree. Unfortunately, the wall chart was never published but the idea of a route map that would show the relationship between various alloy types remained. Inevitably, because Metrode’s product range was dominated by stainless steels and nickel-base alloys, this particular emphasis has been retained.
This small book is the direct result of those early developments and the original name has been retained in the title The alloy tree: A guide to low- alloy steels, stainless steels and nickel-base alloys. It is intended to be a broad introduction to many of the alloys used in petrochemical, power generation and oil and gas engineering. It is not designed to be a formal textbook, but is more of a general guide to the more commonly used alloys and will be of value to the engineer with an interest in the alloy materials available, as well as the emerging metallurgist who has an interest in the field of alloy devel- opments and their areas of application.
Those who are already familiar with the major reference books, some of which are listed in the bibliography, will realise that this book does no more than scratch the surface. Nevertheless, in describing about 100 alloys, it covers a wide range of applications. Inevitably, boundaries have to be defined and this book deals with iron-base and nickel-base systems, and the interaction between the two.
It does not deal with light alloys based on aluminium, magnesium or titanium. At the two extremes of the alloy system, it does not cover simple carbon or very low-alloy steels in any great detail, nor does it make more than passing reference to the highly specialised area of nickel-base superalloys used in the aerospace industries. Those with a particular inter- est in these excluded groups will have to look elsewhere.
The information given has been obtained from a wide variety of sources, some of the more important of which are given in the bibliography. However, responsibility for the contents lies solely with the author and he accepts full responsibility for any errors and omissions.
J. C. M. Farrar Denby Dale
As mentioned in the Preface, this book is based on a wall chart, designed by the author but never published. It was intended to show the evolution of and relationship between the more important alloy systems in the Metrode range of alloyed welding consumables. This book is also based on the Metrode Technical Handbook, which has been a cornerstone of Metrode’s technical support package for almost 40 years, and for which the author, as Technical Director, was responsible from 1981 to 2000. This book would not have been possible without the considerable help, support and encouragement of col- leagues Adam Marshall, Chief Metallurgist, and Graham Holloway, Techni- cal Support Engineer, who have helped both with the technical content and the proofing of this book.
However, final responsibility for the contents and for any errors or omis- sions rests solely with the author.
The alloy tree
The alloy tree diagram on page xiii provides an overview of the most impor- tant iron-base and nickel-base alloy groups and how they are linked. It starts with plain carbon mild steel at the bottom and illustrates how increas- ing alloy content eventually leads to pure nickel at the top. There are two dis- tinct routes: one up the left hand side, which is based on low- or very low-carbon alloys designed primarily for corrosion resistance in aqueous environments, and one up the right hand side which is based on controlled carbon or high-carbon alloys designed primarily for resistance to high tem- peratures in a range of atmospheres. There are other branches, which deal with low-alloy creep-resisting and cryogenic steels.
There are ten alloy groups designated as Groups A to J. The route map within each group shows the detailed relationships between closely related alloys. The route maps also show, in general terms, the changes in alloy content between one alloy and the next. Each alloy, or group of very closely related alloys, carries a reference code, which is the group reference letter, com- bined with a unique number, and this is the link to each individual data sheet (A–0, A–1, A–2, etc). A very few alloys, which tend to be generic groups in their own right, do not have reference numbers. This means that there is no data sheet but a brief explanation is given in the introduction to each group.
The data sheets are not intended to cover all the detailed information about the properties of a specific alloy. This information is readily available from standard reference books and manufacturer’s literature. They do provide a typical composition and some of the more commonly used specifications and proprietary grades, where applicable. Also included is a description of the alloy, some background and history to the alloy development, and key properties relevant to its application. There is also a section on the more important applications and cross-references to other related alloys or
How to use this guide
xii How to use this guide
applications. The data sheets are deliberately presented in a narrative style, in the hope that the reader will find this less intimidating than a formal data sheet with a mass of numerical data.
It should be noted that in some of the data sheets the header gives a slightly different composition from that shown in the body of the data sheet. The header shows that which is most widely recognised and is in common usage, whereas the compositions given in the sheet are typical mid-range specification values.
Nickel, nickel–copper & nickel–molybdenum
alloys Group J
Corrosion-resistant nickel alloys
The alloy tree, showing the relationships between the major alloy groups.
This page intentionally left blank
0.1C–11Cr–Nb–V–N (up to 3Co)
Low C, + Nb, N & Co for better weldability
+ 1–2% W for even greater creep strength
+ Nb, V & N for improved creep strength
+Cr for hydrogen and corrosion resistance
+C, Cr, W & V for improved creep strength
+Cr & Mo for creep resistance
+Mo for creep resistance
+V for creep resistance
Chrome–moly– vanadium steels
STARTING POINT Plain carbon steel
½ to 3%
The starting point for Group A is plain carbon steel with a carbon content of about 0.2% and essential deoxidants such as manganese and silicon. This composition gives a pearlitic structure of modest strength designed pri- marily for use at ambient temperatures. This group demonstrates the effect of increasing alloy content to improve high-temperature creep performance. It illustrates the evolution from a very simple steel with 0.5% molybdenum, designed for service up to about 450 °C, through to the latest 9 and 12% chromium–molybdenum alloys with complex microalloying, designed for very long-term, high-pressure service at temperatures above 600 °C.
Microstructures change from tempered bainite at the lowest alloy content, through to very strong, tough, tempered martensite with complex carbides and carbonitrides. The most highly alloyed grades, with 12% chromium, are at the threshold of stainlessness, but their application, rather than their composition, means that they are correctly included in this group.
There are a number of side branches, describing steels which do not fall naturally on the main alloy branch, but which are also low-alloy high- temperature steels.
0.2% carbon, 1% manganese, 0.5% molybdenum fine-grained elevated temperature steel Also known generically as P1 steels
This steel is a very simple and economic development of plain carbon man- ganese steels where the addition of only 0.5% molybdenum has a significant effect on high-temperature properties. A typical composition is:
C Mn Mo Si S P Al
Weight % 0.15 1 0.5 0.3 <0.02 <0.02 0.05
This steel is normally supplied in accordance within one of many national and international standards, a few examples of which are given below:
UNS ASTM EN
K12822 Gr. P1 1.5415 K11522 K12821 J12522
These steels are usually supplied in the normalised and tempered (N + T) condition to ensure a fine-grained microstructure with some matrix strengthening and some carbides.
Carbon manganese steels represent the most cost-effective method of alloy- ing, to achieve reasonable strength and toughness combined with good weldability but the addition of only about 0.5% molybdenum gives some improvements in higher-temperature performance and represents the first stage in the evolution of more highly alloyed chrome–molybdenum and chrome–molybdenum–vanadium creep-resisting steels.
The addition of about 0.5% molybdenum provides a degree of matrix strengthening and a modest increase in strength over the plain carbon– manganese steels. However, the real improvement comes in achieving and retaining tensile strength and providing reasonably good creep strength at temperatures up to about 450 °C. This is still well below that required for modern steam-generating plant but represents a useful improvement over carbon–manganese steels at a very modest cost premium. The molybdenum content also enhances resistance to hydrogen attack.
These steels are used primarily for the manufacture of process vessels and associated pipework in chemical and oil refinery process plant. They are used for plant operating at modest temperatures often with hydrogen present and offer good creep resistance and ductility at temperatures not exceeding 400–450 °C. For more demanding conditions, higher-alloyed steels would be used.
11/4% chromium–1/2% molybdenum and 21/4% chromium–1% molybdenum creep-resisting steels Also known generically as Grades P11 or P12 and P21 or P22
These steels are plain chromium–molybdenum creep-resisting steels with no additional strong carbide formers. Typical compositions are:
C Mn Si S P Cr Mo
Weight % P11 0.15 0.5 0.3 <0.02 <0.02 1.25 0.5 P22 0.07 0.6 0.3 <0.02 <0.02 2.25 1
The steels are normally supplied in accordance within one of many national and international standards, a few examples of which are given below:
UNS ASTM EN
P11 K11597 Gr. 11 & 12 1.7355 J12072
P22 K21590 Gr. 21 & 22 1.7383 J21890
These steels are typically supplied in the normalised and tempered con- dition and, if subjected to fabrication and welding are usually retempered at about 690 °C. The resultant microstructure is tempered medium carbon bainite with no retained ferrite.
These plain chrome–moly creep-resisting steels are the simplest of the true creep-resisting steels in this group. They rely on matrix strengthening from the chromium and molybdenum and on the same elements to provide car- bides for grain boundary and dislocation pinning. These steels were devel- oped in the early part of the 20th century and were the ‘workhorse’ steels used in modern fossil-fuelled power generation plant for many decades until the development and introduction of P91 steels during the late 1970s (A–3).
These steels are designed for very long-term service in the creep range at temperatures up to about 560 °C and some components and pipework have been in service for more than 250 000 hours (>30 years). However, their creep strength is quite modest when compared with modern advanced steels and this has resulted in the use of very thick-walled components in order to give the necessary performance with high temperatures and pressures. For example, power station main steam pipes often have a wall thickness in excess of 100 mm with obvious implications in terms of fabrication, repair, handling and support costs.
The main areas of application are steam-generating plant including piping, turbine casings, steam chests, valve bodies and boiler superheaters.
These steels are also widely used in oil refineries and provide good cor- rosion resistance against sulphur-bearing crude oils at 250–450 °C. They are also used in the chemical and petrochemical industries because of their resistance to hydrogen attack and blistering at temperatures up to about 450 °C. Typical applications are hydrocrackers, coal liquefaction plant and ammonia pressure vessels.
These steels and welded joints can suffer from temper-embrittlement after long periods of high-temperature service, which results in embrittle- ment and a risk of low-temperature brittle fracture…